Advances in Condensed Matter Physics

Volume 2013 (2013), Article ID 191282, 4 pages

http://dx.doi.org/10.1155/2013/191282

Research Article

Influence of Excitation Frequency on Raman Modes of Thin Films

A. Dixit,¹ J. S. Thakur,² V. M. Naik,³ and R. Naik²

¹Center in Energy & ICT, Indian Institute of Technology Jodhpur, Rajasthan 342011, India

²Department of Physics and Astronomy, Wayne State University, Detroit, MI 48202, USA

³Department of Natural Sciences, University of Michigan-Dearborn, Dearborn, MI 48128, USA

Received 29 July 2013; Accepted 9 September 2013

Academic Editor: David Huber

Copyright © 2013 A. Dixit et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Low energy optical modes of MBE-grown thin films with different values of are investigated using Raman spectroscopy. We also studied the influence of Raman excitation frequency using red and green lasers on scattering intensity of various Raman modes. For those alloys whose bandgap energy is close to the red laser, a huge enhancement in the intensities of A₁(LO) mode and its 2A₁(LO) replica is observed when excited with red laser as compared to the green laser excitation. We found that the energies of longitudinal optical modes (A₁(LO) and 2A₁(LO)) vary nonlinearly unlike the E₂ mode with increasing Ga atomic fraction. A Raman mode ~540 cm⁻¹ was observed in all films with low energy red laser excitation but was absent with green laser excitation. We attribute this mode to A₁(TO) mode of the underneath GaN buffer layer.

1. Introduction

Currently various optical properties of alloys are extensively studied because of their potential applications in full-solar-spectrum photovoltaics [1–3], high-performance light-emitting and laser diodes [4, 5], and solid-state lighting [6]. In addition to the investigation of their bulk properties, the quantum well structures of these alloys are also currently investigated for a variety of applications including laser diodes and -photoluminescence spectroscopy with InGaN quantum disks [7]. High efficiency quantum well structure light-emitting-diodes in the blue-green region of the spectrum and laser diodes emitting violet light have already been made from group-III nitride semiconductors [8, 9] and are in commercial use. In all these devices forms an active layer. The bandgap of these alloys can also be tuned from near-infrared (IR) to ultraviolet (UV) regimes, and in addition these alloys can be fabricated to further increase their bandgap energy by quantum confinement effects [10].

Photoluminescence and other optical properties are strongly influenced by electron relaxation rates due to electron-electron and electron-phonon scattering [11, 12]. So it is important to investigate their various phonon modes and how their spectral features can be influenced by the source excitation frequency. We studied the phonon modes of alloys using Raman spectroscopy and variations in their energies with increasing Ga atomic fraction in the InN compound matrices. We also investigated the effects of Raman excitation frequency on the scattering intensity of these modes for various values of .

2. Experiment

thin films with = 0, 0.15, 0.30, and 0.54 were prepared by MBE [13, 14] technique. Thin buffer layers of AlN and GaN with thickness ~10 nm and 220 nm were grown to reduce the lattice mismatch between thin films and c-sapphire substrate. The thickness of the layer is ~0.6 μm. The carrier concentrations and Hall mobilities of these thin films were determined at room temperature using Van der Pauw method, and their values are listed in Table 1. We notice a small increase in carrier concentration and a substantial decrease in mobility with increasing Ga atomic fraction in the films. The well-defined interference fringe width from UV-Vis-NIR reflection spectrum was used to estimate the thickness of these thin films whose values are given in Table 1.

Table 1: Room temperature electronic and optical properties of thin films.

Sample
Thickness (μm)
Bandgap (eV)
Carrier concentration (cm⁻³)
Mobility (cm²/V·s)
Probing depth (μm) for laser excitation used

514 nm
785 nm

GS1814 InN
0.6
0.77
1.3 × 10¹⁸
900
<0.03
0.06

GS1651 In0.85Ga0.15N
0.5
0.96
1.43 × 10¹⁸
700
<0.03
0.06

GS1942 In0.70Ga0.30N
0.5
1.27
2.3 × 10¹⁸
140
<0.03
0.07

GS1651 In0.46Ga0.54N
0.4
1.85
1.1 × 10¹⁸
20
0.06
0.16

3. Results and Discussion

A strong electron-phonon Fröhlich interaction in wurtzite crystals can lead to a large enhancement in light scattering by polar LO phonons when an incident photon’s energy is close to band gap energy of semiconductor [15, 16]. In many cases it has also led to excitation of replica phonon modes. In wurtzite structure, there are six Raman active modes, E₂(low), E₂(high), A₁(TO), A₁(LO), E₁(TO), and E₁(LO) [17, 18], which are observed in the first order Raman spectrum of films. Other optical modes, B₁(low) and B₁(high), are silent in wurtzite nitrides but are occasionally observed in disordered films [19]. In this paper, we investigated the role of excitation energy on the Raman intensity of these modes by choosing two laser energies, the green laser (514.5 nm = 2.41 eV) having energy larger than the bandgap energy of all the films we have studied here and the red laser (785 nm = 1.58 eV) having energy between the band gap energy of = 0.3 film ( = 1.30 eV) and of = 0.54 film ( = 1.85 eV). Out of the six Raman active modes, we observed E₂(high) and the first-order A₁(LO) Raman modes when the samples were excited by red laser (Figure 1). Along with these modes, 2A₁(LO) replica mode is also observed in all the samples. In between E₂(high) and A₁(LO) modes, one can also see a mode around 540 cm⁻¹ in all the films. A similar mode has been observed [20] in postannealed InN thin films and has been marked as an unidentified feature. However, we associate this mode with A₁(TO) mode of GaN originating from the GaN buffer layer used in all the films. This mode is not observed with green laser (Figure 2(a)) because of the stronger absorption of the green laser by the top layer. We have used the absorption coefficients given in [21] to estimate the probing depth 1/2α, where αis the absorption coefficient. The probing depths for the two excitation laser wavelengths used in the present work (514.5 and 785 nm) are reported in Table 1. Clearly, the probing depth is larger at 785 nm laser excitation compared to that of 514.5 nm for all the samples. Further, the probing depth increases with increasing Ga concentration and substantiates the strong absorption of high energy 514.5 nm photons in the upper layers compared to the low energy 785 nm photons which are transmitted into the lower GaN buffer layer. As Ga atomic fraction in is increased, the energies of these modes (E₂(high), A₁(LO), and 2A₁(LO)) increase as shown in Figure 3(a), as expected. However, there is a dramatic decrease in the intensity of E₂(high) mode relative to A₁(LO) mode accompanied by an increase in damping due to increase in the lattice disorder from Ga atoms substitution. At = 0.54, E₂(high) mode has almost disappeared into the noise. With increasing value, the absorption of the laser energy decreases in the layer due to increase in the bandgap values and at = 0.54, the bandgap value ( = 1.86 eV) of layer becomes larger than the laser energy. This leads to a stronger transmission of the laser energy into the subsequent layers, GaN and sapphire layers, and as a result intense excitations of many sapphire modes as marked by circles along with the A₁(TO) of GaN marked as (top panel, = 0.54 in Figure 1). We also observed an intense structure at 1070 cm⁻¹. Similar structure, however with less intensity, has been associated with the combination of (432 cm⁻¹) GaN mode and (645 cm⁻¹) sapphire mode [22]. Because of stronger excitation of the sapphire modes in this film, the observed mode could be a result of this combination.

Figure 1: Raman spectra of ( = 0, 0.15, 0.30, and 0.54) thin films using red laser excitation source (785 nm = 1.58 eV). The dashed lines are guides to eyes tracing variation of A₁(LO) and its replica 2A₁(LO) mode with increasing Ga atomic fraction. The asterisk (red) indicates the A₁(TO) GaN mode, and circles show the sapphire modes observed in In0.46Ga0.54N thin films (colored online).

(a)

(b)

Figure 2: (a) Raman spectra of ( = 0, 0.15, 0.30, and 0.54) thin films and (b) variation in the energy of E₂(Low) using green laser excitation source (514.5 nm = 2.41 eV). The dashed lines are guides to eyes tracing variations of E₂(low) and A₁(LO) and its replica 2A₁(LO) mode energies with increasing Ga atomic fraction.

(a)

(b)

Figure 3: (a) Energy variations of 1A₁(LO), 2A₁(LO), E₂(Low), and E₂(high) modes with respect to Ga atomic fraction in alloy thin films. (b) Variation in the ratio of A₁(LO)/E₂(high) with respect to Ga atomic fraction for alloy thin films for red and green lasers (Colored online), inset showing bandgap variation with respect to Ga atomic fraction for alloy thin films.

In Figure 2(a) we show the Raman spectra of films when excited off-resonance with green laser. A big change in the Raman intensities of these modes is observed when compared with the corresponding Raman spectral intensities obtained using red laser. The green laser energy is larger than the bandgap energies of the films, so there will be a negligible transmission of green laser energy into the GaN buffer layer underneath the films and sapphire substrate. As a result, no sapphire and GaN modes are observed in thin films with green laser, as shown in Figure 2(a). With increasing atomic fraction of Ga, the bandgap energy of layer increases and begins to tune with the laser energy. This increases the Fröhlich electron-phonon interaction leading to a stronger excitation of A₁(LO) and 2A₁(LO) phonons. At = 0.54, the A₁(LO) and 2A₁(LO) phonons become quite intense compared to the E₂ modes. On the contrary, the Raman intensities of E₂(low) and E₂(high) modes decrease with increasing values of x and at = 0.54; these modes cease to exist due to overdamping by the substitutional disorder of Ga atoms. Note that E₂(low) mode could not be observed when excited with red laser. In Figure 2(b), we also show the shift in the energy of E₂(low) mode with increasing values of . The energies of the observed A₁(LO) and 2A₁(LO) modes increase nonlinearly (Figure 3(a)), while those of E₂ modes vary almost linearly with increasing Ga atoms concentration. We attribute this nonlinear behavior to the c-axial strain in our films due to their small thickness affecting lattice polarization along the c-axis more than in other directions [23]. Similar behavior of these modes is also observed for the red laser when Ga concentration is increased. Figure 3(b) shows variation in the relative intensities of A₁(LO) and E₂(high) modes for red and green lasers. The inset in Figure 3(b) shows the variation of the energy bandgap of thin film samples as a function of Ga atomic fraction x. Clearly the ratio A₁(LO)/E₂(high) is quite large for red laser and varies quite strongly as compared to that of the green laser with increasing concentration of Ga. At a particular value of x, there is no change in the frequency of these modes when energy of the laser is changed; however, the intensities of some of the modes change dramatically.

4. Summary

In summary, we have investigated the intensity of Raman scattering in thin films when their bandgap energy is close to the excitation frequency of the laser. We found that tuning of electronic bandgap transition of the films with the laser excitation frequency dramatically influences the scattering intensities of A₁(LO), 2A₁(LO), E₂(Low), and E₂(high) modes.

Acknowledgment

The authors thank Dr. W. J. Schaff for providing the samples used in this work.

References

J. Wu, W. Walukiewicz, K. M. Yu et al., “Superior radiation resistance of alloys: full-solar-spectrum photovoltaic material system,” Journal of Applied Physics, vol. 94, no. 10, pp. 6477–6482, 2003.

J. Wu, W. Walukiewicz, W. Shan et al., “Effects of the narrow band gap on the properties of InN,” Physical Review B, vol. 66, no. 20, Article ID 201403(R), 4 pages, 2002.

T. Kuykendall, P. Ulrich, S. Aloni, and P. Yang, “Complete composition tunability of InGaN nanowires using a combinatorial approach,” Nature Materials, vol. 6, no. 12, pp. 951–956, 2007.

F. A. Ponce and D. P. Bour, “Nitride-based semiconductors for blue and green light-emitting devices,” Nature, vol. 386, pp. 351–359, 1997.

S. Nakamura, S. Pearton, G. Pearton, and G. Fasol, The Blue Laser Diode: The Complete Story, Springer, Berlin, Germany, 2000.

E. F. Schubert and J. K. Kim, “Solid-state light sources getting smart,” Science, vol. 308, no. 5726, pp. 1274–1278, 2005.

S. Nakamura, M. Senoh, S. Nagahama et al., “InGaN-based multi-quantum-well-structure laser diodes,” Japanese Journal of Applied Physics 2, vol. 35, no. 1, pp. L74–L76, 1996.

S. Nakamura, “InGaN-based violet laser diodes,” Semiconductor Science and Technology, vol. 14, no. 6, article R27, 1999.

S. Nakamura, “InGaN/AlGaN blue-light-emitting diodes,” Journal of Vacuum Science and Technology A, vol. 13, no. 3, article 705, 6 pages, 1995.

H. J. Xiang, S. H. Wei, J. L. F. Da Silva, and J. Li, “Strain relaxation and band-gap tunability in ternary nanowires,” Physical Review B, vol. 78, no. 19, Article ID 193301, 4 pages, 2008.

J. S. Thakur, Y. V. Danylunk, D. Haddad, V. M. Naik, R. Naik, and G. W. Auner, “Transmission phase shift of phonon-assisted tunneling through a quantum dot,” Physical Review B, vol. 77, no. 3, Article ID 035309, 8 pages, 2007.

J. S. Thakur, G. W. Auner, D. B. Haddad, R. Naik, and V. M. Naik, “Disorder effects on infrared reflection spectra of InN films,” Journal of Applied Physics, vol. 95, no. 9, pp. 4795–4801, 2004.

H. Lu, W. J. Schaff, J. Hwang, H. Wu, G. Koley, and L. F. Eastman, “Effect of an AlN buffer layer on the epitaxial growth of InN by molecular-beam epitaxy,” Applied Physics Letters, vol. 79, no. 10, pp. 1489–1491, 2001.

H. Lu, W. J. Schaff, J. Hwang, H. Wu, G. Koley, and L. F. Eastman, “Effect of AlN buffer layer on the epitaxial growth of InN by molecular-beam epitaxy,” Applied Physics Letters, vol. 79, no. 10, pp. 1489–1491, 2001.

C. Chen, M. Dutta, and M. A. Stroscio, “Electron scattering via interactions with optical phonons in wurtzite crystals,” Physical Review B, vol. 70, no. 7, Article ID 075316, 7 pages, 2004.

B. C. Lee, K. W. Kim, M. A. Stroscio, and M. Dutta, “Optical-phonon confinement and scattering in wurtzite heterostructures,” Physical Review B, vol. 58, no. 8, pp. 4860–4865, 1998.

Z. G. Qian, W. Z. Shen, H. Ogawa, and Q. X. Guo, “Experimental studies of lattice dynamical properties in indium nitride,” Journal of Physics: Condensed Matter, vol. 16, no. 12, pp. R381–R414, 2004.

H. Harima, “Properties of GaN and related compounds studied by means of Raman scattering,” Journal of Physics: Condensed Matter, vol. 14, no. 38, p. R967, 2002.

V. Y. Davydov, V. V. Emtsev, I. N. Goncharuk et al., “Experimental and theoretical studies of phonons in hexagonal InN,” Applied Physics Letters, vol. 75, no. 21, pp. 3297–3299, 1999.

J. W. Pomeroy, M. Kuball, C. H. Swartz, T. H. Myers, H. Lu, and W. J. Schaff, “Evidence for phonon-plasmon interaction in InN by Raman spectroscopy,” Physical Review B, vol. 75, no. 3, Article ID 035205, 6 pages, 2007.

J. Wu, W. Walukiewicz, K. M. Yu et al., “Small band gap bowing in alloys,” Applied Physics Letters, vol. 80, no. 25, pp. 4741–4743, 2002.

H. W. Kunert, J. Barnas, D. J. Brink, and J. Malherbe, “Raman active modes of one-, two-, and three-phonon processes in the most important compounds and semiconductors with the rhombic, tetragonal, regular, trigonal, and hexagonal structures,” Journal de Physique IV, vol. 132, no. 1, pp. 329–336, 2006.

D. Cai and G. Y. Guo, “Tuning linear and nonlinear optical properties of wurtzite GaN by c-axial stress,” Journal of Physics D, vol. 42, no. 18, Article ID 185107, 2009.